J Wood Sci (1999) 45:127-133 © The Japan Wood Research Society 1999
Song-Yung Wang • Hou-Lin Wang
Effects of moisture content and specific gravity on static bending properties
and hardness of six wood species*
Received: May 26, 1998 / Accepted: September 18, 1998
Abstract This study was designed to investigate the effects of moisture content (MC) and specific gravity (SG) on the bending strength and hardness of six wood species including Japanese cedar
(Cryptomeria japonicaD. Don), China fir
(Cunninghamia lanceolata),western hemlock
(Shoreaspp.), Selangan batu
(Shoreaspp.), and red oak
(Quercusspp.). The experimen- tal results are summarized as follows: Effects of MC and SG on the strength (MOR), stiffness (MOE), and hardness (HB) could be represented by a multiregression formulas. A negative correlation existed between these properties and MC, whereas a postive correlation showed between them and the SG. The changing rate of these properties induced by 1% MC changes varied with the wood species: 2.6% change in M O R was observed in Japanese cedar, China fir, western hemlock, red meranti, and Selangan batu; and 3.9 % was found in red oak. For MOE, a 0.58% change was observed in Japanese cedar, China fir, and red meranti; western hemlock and Selangan batu exhibited 1.2% and red oak 2.5%. For hardness, a 1.1% change was observed in Japanese cedar, western hemlock, and red oak; red meranti and China fir exhibited 3.3%; and Selangan batu 1.8%. Key words Moisture content • Specific gravity - Strength • Stiffness • Hardness
It is well known that wood is a hygroscopic, elastic material; hence its mechanical properties are highly affected by the
S.-Y. Wang ( ~ ) • H.-L. Wang
Department of Forestry, College of Agriculture, National Taiwan University, No. 1, Sec. 4, Roosevelt Road, Taipei, Taiwan, ROC Tel. +886-2363-1736; Fax +886-2-23631736
* A part of this report was presented at the 48th annual meeting of the Japan Wood Research Society in Shizuoka, Japan, April 3-5, 1998
change of its moisture content (MC). In general, most me- chanical properties of wood vary inversely with the MC of the wood below the fiber saturation point (FSP). It was reported that the average changing rates for the static bending modulus of elasticity (MOE), modulus of rup- ture (MOR), compression parallel-to-grain, and hardness of certain clear wood can be approximated, respectively, as 2%, 4%, 6%, and 2.5% for 1% MC change below FSP at a constant temperature of 70°F (21.1°C). Furthermore, a logarithm formula representing the strength-MC relation for wood with MC below the FSP was also developed by Forest Products Laboratory (FPL) ~ in which variables such as the strength of wood at an MC of 12% and green condi- tion, as well as a specific value of MC, at which the wood strength begin to change when drying from the green condi- tion was considered. That formula provided more accurate prediction of the strength-MC relations of wood, but the specific values of MC were reported for only 13 wood spe- cies. Therefore, in this study the effect of MC (below FSP) on the static bending properties and hardness of six wood species was closely examined statistically. Mean values for more accurate prediction of the strength changing rate as affected by the moisture fluctuation are presented. Further- more, the interrelation among the mechanical properties, moisture content, and specific gravity was statistically analyzed.
Materials and methods
Table 1. Temperature and relative humidity conditions for designated equilibrium moisture content
Condition no. Dry bulb Difference between dry and Relative humidity (%) Extimated moisture content (%)
temperature (°C) wet bulb temperature (°C)
1 20.00 0.23 98.00 25.00
2 20,00 1.22 89.00 20.00
3 20,00 2.60 77.20 15.00
4 20.00 5.43 54.79 10.00
5 20.00 9.80 24.30 5.00
6 20.00 14.07 0 0
The dimensions of specimens for static bending were 37cm (long, in longitudinal direction) × 3 c m (width) × 1.5cm (thick) and 4 c m (long, in longitudital direction) × 3 c m (width) × 1.5cm (thick) for the hardness test.
Adjustment of MC of tested specimens
The M C of specimens was one of the major variables in this study. The designated six M C levels ranged from 0% to 25% at intervals of 5%. The constant temperature and rela- tive humidity ( R H ) conditions for obtaining the equilibrium moisture content (EMC) are given in Table 1. Conditions 1 to 4 (MC levels: 25%, 20%, 15%, and 10%) were controlled using conditioning chambers with a constant temperature of 20°C; and their R H s were set at the levels of 98%, 89%, 77.2%, and 54.79%, respectively. However, conditions 5 and 6 (i.e., M C 5% and 0%) were obtained using the con- centration of sulfuric acid solution in a desiccator under a constant temperature of 20°C. 2 The concentrations of sulfu- ric acid solution were 56.63% and 100% for conditions 5
and 6, respectively. All specimens were conditioned about 2
months until they reached their EMC.
Static bending tests
The static bending test was conducted in accordance with the central concentration loading m e t h o d ] A Shimadzu model U H - 1 0 A testing machine was used. The span/depth ratio was 14 for all specimens. The average crosshead was 150 kgf/cm2/min of bending strength. The proportional limit and ultimate load and deflection were recorded, and the M O E and M O R were calculated.
The hardness test was conducted in accordance with the Brinell hardness method. 4 T h e Brinell hardness of tangen- tial sections of specimens (HB) was calculated f r o m the following formula
H13 = P/IO ( k g f / m m 2) (1) where P represents the corresponded loading with 1/rcmm of the press depth of the steel ball ( 1 0 m m in diameter). The
Table 2. OD-based specific gravity of six wood species
Wood species ,0o Coefficient of
China fir 0.33 _+ 0.012 3.6
Japanese cedar 0.38 _+ 0.027 7.1
Western hemlock 0.45 _+ 0.033 7.3
Red oak 0.66 _+ 0.029 4.4
Red meranti 0.48 _+ 0.045 9.4
Selangan batu 0.90 +_ 0.048 5.3
There were 30 samples of each wood species. ,Oo, specific gravity (results are the means + SD).
O D - b a s e d specific gravity (0o) and M C were obtained using the specimens cut from both ends (dimension 4 × 3 × 1.5 cm) of the bending specimens.
Results and discussions
Oven-dried-based specific gravity
The oven-dried ( O D ) - b a s e d specific gravity for each w o o d species (0o) obtained under the designated six conditions are given in Table 2. It was found that the Qo value for China fir was lowest, and largest value was found for Selangan batu. The lowest variation coefficient (CV) occurred in China fir specimens, and a higher variation was seen in red meranti.
Relations between humidity conditioning and moisture contents
The protocol used by Forest Products L a b o r a t o r y - US. D e p a r t m e n t of Agriculture ( F P L - U S D A ) for conditioning the M C of spruce w o o d was adapted for controlling temperature and R H in this study. However, the M C of specimens tested was not in full agreement with the values as described in the F P L observation and certainly varied with the w o o d species. Because the constant temperature was controlled at 20°C in this study, the R H was considered to be the sole affecting factor. Their relations could be represented by the following exponential formulas; and five other w o o d species showed a similar trend:
China fir: M C = 3.26e °'°2°Rn r = 0.98** (2)
W e s t e r n hemlock: M C = 2.41e °°26RH r = 0.97** (4)
R e d oak: M C = 2.58e °°23RH r = 0.94** (5)
R e d meranti: M C = 2.39e °°25RH r = 0.96** (6)
S e l a n g a n batu: M C = 2.95e °°22RH r = 0.95** (7)
w h e r e the d o u b l e asterisk (**) indicates g r e a t significance resulted f r o m the F - v a l u e test at the 0.01 confidence level, which m e a n s that the E M C of w o o d could b e p r e d i c t e d by the R H in a c o n s t a n t - t e m p e r a t u r e e n v i r o n m e n t . 57 W h e n the R H was set at 0 in these e x p o n e n t i a l formulas, the E M C values were n o t equal to 0. This m a y b e a t t r i b u t e d to the fact that the conditions of 0% and 24.3% R H were main- t a i n e d using sulfuric-acid solution, and it m a y b e not e n o u g h to p r o v i d e a c o m p l e t e l y e q u i l i b r a t e d c o n d i t i o n for the dura- tion of 2 months. H o w e v e r , w h e n R H was set at 100%, E M C r e a c h e d the F S P values of that w o o d species. T h e F S P s of six w o o d species c a l c u l a t e d f r o m the a b o v e f o r m u - las w e r e 25.1% for C h i n a fir, 28.5% for J a p a n e s e cedar, 33.8% for w e s t e r n h e m l o c k , 24.5% for r e d oak, 30.0% for r e d m e r a n t i , and 27.4% for Selangan batu. It was f o u n d that in coniferous w o o d the F S P values i n c r e a s e d with an in- c r e a s e in their 0o values. In decreasing order, it was W e s t e r n h e m l o c k > J a p a n e s e c e d a r > China fir. This is in a g r e e m e n t with a previous r e p o r t 8, in which an F S P value of 3 1 . 1 % - 34.0% for J a p a n e s e cedar, and 2 6 . 2 % - 2 9 . 2 % for China fir were o b s e r v e d using the shrinkage m e a s u r e m e n t m e t h o d s ; W e s t e r n h e m l o c k was n o t i n v e s t i g a t e d in that study.
W a n g and Cho 9 c o n d u c t e d the d e s o r p t i o n and a d s o r p - tion e x p e r i m e n t at constant t e m p e r a t u r e s of 20 ° , 30 ° , and 40°C, u n d e r various R H conditions. F r o m the hygroiso- t h e r m of 20°C, E M C values o b s e r v e d at the 100% R H c o n d i t i o n were c o n s i d e r e d to b e the FSP. W i t h this ap- p r o a c h , values of 29.70% and 29.65% w e r e o b t a i n e d f r o m d e s o r p t i o n conditions and 28.96% and 29.93% during ad- s o r p t i o n for J a p a n e s e c e d a r and s o u t h e r n r e d oak, respec- tively. T h e results for J a p a n e s e c e d a r in that study w e r e close to those of this study, but the value for s o u t h e r n r e d o a k was slightly h i g h e r t h a n that f o u n d in this study.
Effects of m o i s t u r e c o n t e n t and specific gravity on M O R
It is well k n o w n that the static strength of w o o d is affected b y m a n y factors, including m o i s t u r e content, specific grav- ity, grain angle, and the width of the a n n u a l ring and knots. In this study, m o i s t u r e c o n t e n t was c o n s i d e r e d to be the p r i n c i p a l variable for investigating the effect of M C levels on static b e n d i n g strength. It was f o u n d that M O R values d e c r e a s e d linearly with the increase of M C a n d could b e e x p r e s s e d by the following l i n e a r regression formulas:
M O R = 972.88 - 18.31MC, r = 0.76** (8)
J a p a n e s e cedar:
M O R = 897.67 - 15.27MC, r = 0.64** (9)
W e s t e r n h e m l o c k :
M O R = 1195.68 - 22.70MC, r = 0.91"* (10)
R e d oak:
M O R = 1409.19 - 31.46MC, r = 0.85** (11)
R e d meranti:
M O R = 1605.52 - 16.37MC, r = 0.64**
M O R = 2333.39 - 51.00MC r = 0.79**
A l t h o u g h the a b o v e - l i s t e d c o r r e l a t i o n coefficients (r) are n o t v e r y high, highly significant differences (0.01 confidence level, **) existed as shown in an F-value test. F u r t h e r exami- n a t i o n of the e x p e r i m e n t a l d a t a i n d i c a t e d that the v a r i a t i o n of specific gravity within an individual w o o d species was large; h e n c e specific gravity was n o t c o n s i d e r e d a d e p e n d e n t variable, w h e r e a s the r e l a t i o n b e t w e e n specific strength MOR/,o o and M C was c o n s i d e r e d to be. T h e y can be e x p r e s s e d as follows:
M O R / 0 o = 268577 - 1526.93MC, r = 0.45** (14)
J a p a n e s e cedar:
M O R / 0 o = 160891 - 874.08MC, r = 0.17"* (15)
W e s t e r n hemlock:
MOR/~)o = 223352 - 1823.37MC, r = 0.63** (16)
R e d oak:
M O R / 0 o = 185622 - 3239.80MC, r = 0.88** (17)
R e d meranti:
M O R / 0 o = 243395 - 1356.99MC, r = 0.31"* (18)
MOR/Qo = 223901 - 2325.50MC, r = 0.50** (19)
A l t h o u g h the F - v a l u e test i n d i c a t e d that the c o r r e l a t i o n coefficients (r) were greatly significant at the 0.01 level, the resultant r values were p o o r in c o m p a r i s o n with those w h e n the specific gravity was n o t c o n s i d e r e d (i.e., M O R vs. MC). T h e r e f o r e it seems that the specific M O R cannot be used satisfactorily for e x p e r i m e n t a l d a t a analysis. H o w e v e r , much m o r e impressive results were o b t a i n e d w h e n the mul- tivariable analysis 1° was conducted. W h e n M C and Oo are c o n s i d e r e d i n d e p e n d e n t variables, M O R can be e x p r e s s e d by multiregressions formulas as shown in T a b l e 3.
Obviously, the c o r r e l a t i o n coefficients (r), ranging f r o m 0.75 to 0.94, were much m o r e significant t h a n those in the single-variable l i n e a r regression formulas. H e n c e the m u l t i v a r i a b l e regression offers a b e t t e r e x p l a n a t i o n of ma- t e r i a l p r o p e r t i e s analysis w h e n v a r i a t i o n m a y exist. H o w - ever, in the m u l t i v a r i a b l e analysis the i n t e r c o r r e l a t i o n a m o n g d e p e n d e n t variables m u s t not exist, otherwise the analyzed result would be significantly affected. T h e r e f o r e , the O D - b a s e d specific gravity (Qo) was used i n s t e a d of the a i r - d r i e d values (Q) to exclude the M C effect on specific gravity,
F r o m the a b o v e results, a negative c o r r e l a t i o n b e t w e e n M O R and M C a n d a positive c o r r e l a t i o n b e t w e e n M O R and 0o were observed. A l t h o u g h a positive c o r r e l a t i o n be- t w e e n M O R and Qo has b e e n r e p o r t e d by m a n y researchers, their results v a r i e d with w o o d species. ~l-x~
TabLe 3. Coefficients of the multiregression formulas for the relations among MC, ~o, and strength properties of six wood species
W o o d species y = a + b x 1 + cx2
and kinds of
strength a b C r
M O R -460.29 -18.07"* 394.46** 0.93 M O E -44700.1 -538.2** 392005.4** 0.80
HB -0.30 -0.013"* 3.31" 0.58
MOR 213.03 -16.49"* 1814.09'* 0.80
MOE -55359.02 -412.85 310036** 0.82
H B 1.21 -0.011" 25.44** 0.55
MOR 276.09 -21.22"* 1976.13"* 0.94
MOE 60837.79 -914.42"* 2.255 0.71
H B -7.73 -0.029* 52.07* 0.86
MOR 922.76 -31.18"* 736.23 0.84
MOE 10683.05 -2066.73** 92025.04 0.88
H B 19.02 -0.078** 21.57 0.71
MOR 38.74 -16.21"* 2220.38** 0.75
MOE 8868.94 -647.41 28854.12"* 0.51
HB 6.83 -0.0096** 6.81 0.43
MOR -4058.01 -48.72** 7172.78"* 0.93
MOE -497784.9 -1909.96"* 783792** 0.85
HB 22.54 -0.028** 8.41 0.42
y, represents M O R , M O E , and HB, respectively; xz and x 2 shows MC and ~)o, respectively; a, b, c, coefficient for multiregression formulas. *, **, significant (0.05 level) and very significant (0.01 level) by F-tests.
examined using the results of the six w o o d species studied and discussed as follows.
A s s u m e M O R is a function of M C [i.e., M O R = f(MC)]. The M O R changing rate induced by the 1% increase (or decrease) of M C c o m p a r e d to the 12% (air-dried condi- tion) at a condition of M C may be expressed as following formulas:
( d ~ @ c R ) × 1 _ _ _ M O R _ f ( M C )
MOR12 M O R 1 2 M O R ~ 2
_ f ( M C ) (20)
Because six w o o d species were used in this study the regression formulas for M O R and M C were assumed as follows:
MOR1 = f,(MC), M O R 2 = f z ( M C ) . . . MOR6
The M O R changing rate induced by a 1% increase (or decrease) in moisture content for six w o o d species m a y be expressed as follows:
M O R changing rate = ff(MC) f2(MC) .f6'(MC) (22)
f1(12) ' / 2 ( 1 2 ) " ' " f6(12)
If significant differences were not observed among these six wood species as analyzed by D u n c a n s ' multiple new
range method, 17 the variation among them could be neglected. Hence this M O R changing rate should be applicable to all w o o d species; otherwise significant varia- tions among w o o d species cannot be ignored.
Six M C conditions (0%, 5%, 10%, 15%, 20%, 25%) were chosen for the study. These six M C variables were substituted into the regression formula for each wood species, and 36 groups of data were obtained for D u n c a n s ' multiple new-range analysis according to the analyzed result for each w o o d species. If results showed large differ- ences among the changing rates of f'(O)/f(12), f'(5)/f(12),
f'(10)/f(12), f'(15)/f(12), f'(20)/f(12),and
D u n c a n s ' multiple new-range analysis is statistically meanless because of the low F values. That means that the analyzed result would be worthless. Therefore, the function of M O R = f(MC) would be considered efficient. Several functions were used for analysis, and their applicability and suitability were c o m p a r e d each other as follows] s-2°
(1)MOR = f ( M C ) = a - b. M C ( M C < FSP) (23)
This is a popularly used linear regression formula, where a and b are material constants and positive, However, be- cause the M O R changing rate with reference to that at 12% M C is
f ' ( M C ) _ b
f(12) a -+ 12b
it follows that the six w o o d species studied provided data as follows
f ' ( M C / ) _ bi i = 1, 2 .... 6, j = 1, 2 .... 6. (24)
f(12) a i - 12bi'
where i = 1 to i = 6 designate the six w o o d species; and j = i to j = 6 designate the six M C conditions (i.e.,j = 1; M C = 0 % ; . . . j = 6; M C = 25%) and a~ and b, are material constants for the six w o o d species studied. The value of
b](a~ -12bi) is a constant and is wood-species dependent,
but it is independent of MC. Hence D u n c a n s ' multiple new- range analysis could not be conducted.
( 2 ) M O R = f ( ~ ) = a -- b M C -- cM--C 2 o r
c M C + b M C + ( M O R - a ) = 0
physically 0 < M C < FSP (i.e., MC is alway positive and real) and M O R - a < 0 (i.e., M O R -< a, M O R and a, positive and real); hence at MC = 0, MORl~c=0 is the maximum value,
where a, b, and c are material constants, and must be real. Mathematically, there are three possible solutions for this quartic function:
(B) If b 2 -- 4(MOR - a)c < 0, the MC (roots) are imaginary and unequal which is also physically meaningless because MC is alway real. Hence this solution must be excluded.
(C) If b 2 - 4(MOR - a)c = 0, the MC (roots) are real
and equal, which is physically meaningful because only a single value of MC exists for the M O R at that MC condi-
tion. Furthermore, b 2 = 4(MOR - a)c leads to c, which
must be negative and real because M O R - a < 0 for all MC conditions that are less than 0%. It follows that MC must be
equal to - b/2c. Thus b must be positive for a positive value
of MC, and a is a specified value of MOR. This solution is acceptable both mathematically and physically.
Using the argument described above, it follows that the M O R changing rate with reference to that at 12% MC condition for the six wood species had a general form as
f l " ( ~ , ) _ - b i - 2 c i M C i
f(12) a i - 1 2 b i - 144ci
where, i = 1 to i = 6 designates the six wood species, and ] = 1 to j = 6 designates the six MC conditions. Thus the Duncans' multiple new-range analysis could be performed. The results are shown in Table 4.
(3)MOR = ae -'Mc, 0 <_ MC < FSP (26)
where a and b are material constants and positive, and a is the value of M O R at the oven-dried condition. It follows that the M O R changing rate with reference to that at 12% MC for the six wood species studied are
- - - - D i e (27)
The characteristics of this equation are different with that discussed in (2) because it yields only negative values (i.e., - b i < O, b~ is possible).
The M O R changing rate induced by 1% MC fluctuation for six wood species was analyzed using the Duncans' mul-
Table 4. Duncans' multiple new-range test for strength change rate induced by 1% MC change
Wood Rate of change (%) Species
MOR n MOE b HB c
Red meranti 1.92 0.57 3.02
China fir 2.55 0.62 3.49
Japanese cedar 2.70 0.56 1.10
Selangan batu 2.89 1.21 1.83
Western hemlock 2.93 1.20 1.10
Red oak 3.85 2.50 1.11
There were six samples for each determination.
There were no significant differences between the following wood species. MOR: red maranti, China fir, Japanese cedar, Selangan batu, and western hemlock; on between Selangan batu, western hemlock, and red oak. MOE: Japanese cedar, red meranti, and China fir; or between western hemlock and Selangan batu. Hs: Japanese cedar, western hemlock, and red oak; on between red meranti and China fir.
tiple new-range method as shown in Table 4. It is evident from Table 4 that the M O R changing rate was homoge- neous for five wood species (red meranti, China fir, Japa- nese cedar, Selangan batu, and western hemlock) and had an average value of 2.6%; a larger value of 3.9% was seen for red oak. It also was found that the M O R changing rate for the six wood species studied were lower than 4%, which is commonly accepted by the wood science and technology community.
Oda et al. 21 investigated the relations between MC and c~/ja g//(~7/j and a gN represented the compression strength parallel-to-grain in air-dried and water-saturated condi- tions, respectively). Their results indicated that the rela- tions could be represented by a semilogarithmic equation, as shown as
o / / / o g / / = a - blogMC, (0 < MC)
where a and b were constants (positive), and they varied with wood species. However, at the MC range of 11%-19%, the relations between, o~jc~ g// (a15 represented the com- pression strength parallel-to-grain in 15% MC), and MC could be described by a linear regression. The average value of a changing rate for nine conifereous wood species was 6.3%, which was consistent with the value of 6% used in general. However, the study of Oda et al. 2~ showed that the distribution ranged from 4.8% (asunaro) to 7.8% (akamatsu), suggesting that the variation in wood species did exist.
Effects of moisture content and specific gravity on M O E
Results from static bending tests indicated that the relations among MC, ,Oo, and M O E could be represented by the multiregression formula shown in Table 3. It was found that a negative correlation existed between M O E and MC, but there was a positive correlation between M O E and 0o. However, there were no significant effects of MC on M O E in Japanese cedar or red meranti. Similarly, there were no significant effects of ,Oo on M O E in Western hemlock or red oak.
Effects of moisture content and specific gravity on hardness
Results of hardness tests indicated that the relations among
MC, ~Oo, and Brinell hardness (HB) could be represented by
multiregression formulas, as shown in Table 3.
It was found that a negative correlation existed between HB and MC, ranging from significant differences (0.05 level,*) to highly significant differences (0.01 level, **). A positive correlation also existed between H B and ~o, but the differences were not significant for the three hardwoods (red oak, red meranti, and Selangan batu).
T h e HB changing rate induced by 1% M C fluctuation for six w o o d species was analyzed using the same m e t h o d as described above. T h e results of Duncans' multiple new- range test were shown in Table 4. It is evident f r o m Table 4 that the Ha changing rates for Japanese cedar, western hem- lock, and red oak can be classified as a h o m o g e n e o u s group, represented by an average value of 1.1%. Similar trends were showed for red meranti and China fir with an average value of 3.3%. Selangan batu had a value of 1.8%. A value of 2.5% is generally used for the HB changing rate for the longitudinal surface of w o o d (average of radial and tangen- tial faces) induced by 1% M C fluctuation. However, this study suggests that the H B changing rate varied with the wood species.
Correlation a m o n g the three strength properties
1. U n d e r a constant temperature, the M C of w o o d increases exponentially with an increase of RH. That is, the M C of woods could be predicted by the R H in that environment.
2. Effects of M C and Qo on strength ( M O R , M O E , HB) can be represented by multiregression formulas. A negative correlation existed between strength and MC, and a posi- tive correlation existed between strength and ~o.
3. Strength can be assumed as an exponential function of MC, and the strength changing rate induced by 1% M C fluctuation could be obtained by Duncans' multiple new- range analysis. Such rates varied with w o o d species: 2.6% M O R changing rate was observed in Japanese cedar, China fir, western henlock, red meranti, and Selangan batu; it was 3.9% in red oak. M O E changing rate of 0.58% was ob- served in Japanese cedar, China fir, and red oak; it was 1.2% in western hemlock and Selangan batu and 2.5% in red oak. A n HB changing rate of 1.1% was found in Japanese cedar, western hemlock, and red oak; 3.3% in red meranti and China fir; and 1.8% in Selangan batu.
4. Intercorrelatious among M O R , M O E , and HB could be represented by positive linear regression formulas.
Acknowledgments The investigation reported in this paper was sup-ported financially by the National Science Council of the Republic of China (NSC87-2313-B-002-119). The authors thank Dr. R.C. Tang, Professor of the School of Forestry, Auburn University Alabama, USA for his advice.
If the M C of the six w o o d species is neglected, correlations a m o n g three strength properties could be represented by the following positive linear regression formulas:
M O R = 5.04 + 0.0094MOE r = 0.88** M O R = 442.62 + 361.78HB r = 0.73** M O E = 60611 + 28486H B r -= 0.61"*
The correlation coefficients were highly significant at the 0.01 confidence level, as indicated by the F value test, when each w o o d species was considered individually. They also showed positive correlations between M O R and M O E , M O R and HB, and M O E and HB for six w o o d species. Concerning the relation between M O R and M O E , their correlation coefficients ranged from 0.63 (Japanese cedar and red meranti) to 0.87 (red oak). They also were shown to be highly significant (0.01 level) by the F value test. These results are in agreement with results reporetd by m a n y wood researchers. 24-2s However, as to the relation between M O R and HB, their correlation coefficients ranged from 0.31 (red meranti) to 0.86 (western hemlock); and the corre- lation coefficients for M O E and HB ranged from 0.26 (red meranti) to 0.66 (red oak).
Based on the above observations, the following conclusions can be drawn.
1. Wood Handbook 72 (1987) Wood as an engineering material. For- est Products Laboratory, Forest Service, USDA, P4-36-39 2. Forestry and Forest Products Research Institute (1982) Wood In-
dustry Handbook revised 3rd edn, Maruzan Published KK, P1056 3. Chinese National Standard CNS454 (1981) Method of test for static bending of wood. National Standard Bureau, Taipei, Taiwan, ROC
4. Chinese National Standard CNS460 (1981) Method test for hard- ness of wood. National Standard Bureau, Taipei, Taiwan, ROC 5. Avramidis S (1989) Evalvation of "three-variable" models for the
prediction of the equilibrium moisture content in wood. Wood Sci Technol 23:251-258
6, Simpson WT (1971) Equilibrium moisture content prediction for wood. For Prod J 21(5):48-49
7. Simpson WT (1973) Predicting equilibrium moisture content of wood by mathematical models. USDA FPL, Madison, WI 8. Wang SY (1989) Studies on the fundamental properties of the
economical tree species in Taiwan (IV). Q J Chin For 22(1):3-22 9. Wang SY, Cho CL (1993) Equilibrium moisture contents of six
wood species and their influencesl Mokuzai Gakkaishi 39:126-137 10. Hwang CE (1986), Multivarable analysis. Chinese Economic
Enterprise Institute, Taipei, Taiwan, ROC
11. Lin CR, Shih NY, Wang SY (1992) Studies on the lumber grades and bending properties of Japanese cedar and China-fir plantation trees. Q J Exp For NTU6(1):71-101
12. Schneider MH, Sebastian LP (1991) Bending strength and stiffness of Caribbean pine from Trinidad and Tobago. Wood Fiber Sci 23:468-471
13. Wang SY, Tserng WH (1993) Variation in compression parallel-to grain and bending strength of China fir (Cunninghamia lanceolata)
grown in Taiwan. Q J Exp For NTU 7(1):65-77
15. Wang SY, Chiu CM (1993) Wood properties of Japanese cedar originated by seed and vegetative reproduction in Taiwan. VI. Compression and bending properties. Mokuzai Gakkaishi 39:1128-1139.
16. Wang SY, Lin SH (1996) Effects of plantation spacings on the quality of visually graded lumber and mechanical properties of Taiwan-grown Japanese cedar. Mokuzai Gakkaishi 42:435-444 17. Duncan DB (1995) Multiple range and multiple F tests. Biometrics
18. Barett JD, Lau W (1991) Bending strength adjustments for moisture content for structural lumber. Wood Sci Technol 25:433- 447
19. Green DW, Link CL, Debonis AL, Mclain TE (1986) Predicting the effect of moisture content on flexural properties of Southern pine dimension lumber. Wood Fiber Sci 18(1):134-156
20. Green DW, Erans JW, Barrett JD, Aplin EN (1987) Predicting the effect of moisture on the flexural properties of Douglas-fir dimen- sion lumber. Wood Fiber Sci 20(1):107-131
21. Oda K, Tsutsumi J, Matsumura J (i994) Effects of moisture con- tents on mechanical properties of several softwood. II. Effects on
compressive strength and annual ring structure. Mokuzai Gakkaishi 40(2):113-118
22. Gerhard CC (1975) Stress wave and MOE of sweetgum ranging from 150 to 15 percent MC. For Prod J 25(4):51-57
23. Ross RJ, Pellerin RF (1991) NDE of green material with stress waves; preliminary results using dimension lumber. For Prod J 41(6):57-59
24. Atherton GH (1980) Preliminary study of proportional limit as predictor of ultimate strength in bending. For Prod J 30(I1):47-53 25. Faust TD, McAlister RH, Zarnoch SJ (1990) Strength and stiffness properties of sweetgum and yellow-popular structural lumber. For Prod J 40(10):58-64
26. Tanaka T (1988) Evaluation of strength by non-destructive test: application for sugi wood attacked by borer-insect, Wood Ind (Mokuzai Kogyo) 43(2):20-25
27. Wang SY, Ko CY (1998) The dynamic modulus of elasticity and bending properties of large beam of Japanese cedar for Taiwan- grown in different plantation spacing sites. J Wood Sci 44:62-68 28. Zhou H, Smith I (1991) Factors influencing bending properties of